PHYSICAL REVIEW B 86, 125105 (2012)

Spin-orbit tuned metal-insulator transitions in single-crystal Sr2 Ir1−x Rh x O4 (0 x 1) T. F. Qi,1 O. B. Korneta,1 L. Li,1 K. Butrouna,1 V. S. Cao,1,* Xiangang Wan,2 P. Schlottmann,3 R. K. Kaul,1 and G. Cao1,† 1

Center for Advanced Materials and Department of Physics and Astronomy, University of Kentucky, Lexington, Kentucky 40506, USA 2 Department of Physics, Nanjing University, Nanjing, People’s Republic of China 3 Department of Physics, Florida State University, Tallahassee, Florida 32306, USA (Received 28 June 2012; revised manuscript received 8 August 2012; published 6 September 2012) Sr2 IrO4 is a magnetic insulator driven by spin-orbit interaction (SOI) whereas the isoelectronic and isostructural Sr2 RhO4 is a paramagnetic metal. The contrasting ground states have been shown to result from the critical role of the strong SOI in the iridate. Our investigation of structural, transport, magnetic, and thermal properties reveals that substituting 4d Rh4+ (4d 5 ) ions for 5d Ir4+ (5d 5 ) ions in Sr2 IrO4 directly reduces the SOI and rebalances the competing energies so profoundly that it generates a rich phase diagram for Sr2 Ir1−x Rhx O4 featuring two major effects: (1) Light Rh doping (0 x 0.16) prompts a simultaneous and precipitous drop in both the electrical resistivity and the magnetic ordering temperature TC , which is suppressed to zero at x = 0.16 from 240 K at x = 0. (2) However, with heavier Rh doping [0.24 < x < 0.85 (±0.05)] disorder scattering leads to localized states and a return to an insulating state with spin frustration and exotic magnetic behavior that only disappears near x = 1. The intricacy of Sr2 Ir1−x Rhx O4 is further highlighted by comparison with Sr2 Ir1−x Rux O4 where Ru4+ (4d 4 ) drives a direct crossover from the insulating to metallic states. DOI: 10.1103/PhysRevB.86.125105

PACS number(s): 75.70.Tj, 71.30.+h

I. INTRODUCTION

Sr2 IrO4 is an archetype for new physics primarily driven by the interplay of electron-electron and spin-orbit interactions (SOI).1–3 The relativistic SOI proportional to Z 4 (Z is the atomic number) is approximately 0.4 eV in the iridate (compared to ∼20 meV in 3d materials), and splits the t2g bands into bands with Jeff = 1/2 and Jeff = 3/2, the latter having lower energy.1,2 Since the Ir4+ (5d 5 ) ions provide ﬁve 5d electrons, four of them ﬁll the lower Jeff = 3/2 bands, and one electron partially ﬁlls the Jeff = 1/2 band where the Fermi level EF resides. The Jeff = 1/2 band is so narrow that even a reduced on-site Coulomb repulsion U (∼0.5 eV) due to the extended nature of 5d-electron orbitals is sufﬁcient to open a small gap (0.1 eV) supporting the insulating state.1,2 Most recently, an x-ray absorption spectroscopy study indicates a mixing of the Jeff = 1/2 and Jeff = 3/2 bands as a result of exchange interactions (∼0.2 eV) and a tetragonal crystal electric ﬁeld (CEF) (∼0.075 eV).4 Nevertheless, the larger the SOI and the narrower the band is, the smaller U is needed for a SOI-related insulating state,5 in which SOI, Coulomb interactions, tetragonal CEF, and Hund’s coupling JH become so comparable that they vigorously compete with each other, setting a new balance between the relevant energies that can drive new exotic states.1–18 In contrast, the isoelectronic 4d-based Sr2 RhO4 with Rh4+ (4d 5 ) ions with ﬁve 4d electrons has a weaker SOI (∼0.16 eV), thus a smaller splitting between the Jeff = 1/2 and Jeff = 3/2 bands that are more evenly ﬁlled by the ﬁve 4d electrons.5,15–18 The weaker SOI combined with more effectively screened Coulomb interactions between O 2p and Rh 4d electrons favors a metallic state.15 Indeed, Sr2 RhO4 is a paramagnetic, correlated metal16–18 sharply contrasting the magnetic insulator Sr2 IrO4 that orders at TC = 240 K.6,19–21 In addition, comparisons of Sr2 RhO4 with another 4d-based compound, Sr2 RuO4 , a p-wave superconductor, 22 reveal that the impact of the SOI strongly depends on the detailed band structure near the Fermi surface EF , the Coulomb interactions, 1098-0121/2012/86(12)/125105(6)

and the lattice distortions.7,15,23,24 The t2g bands in Sr2 RhO4 near EF are less dispersive than those in Sr2 RuO4 , therefore more susceptible to the SOI-induced band shifts near EF than in Sr2 RuO4 despite the similar strength of the SOI in both materials.23 This is in part because the Ru4+ (4d 4 ) ion has four 4d electrons instead of ﬁve; Ru doping therefore adds holes to the bands. Both Sr2 IrO4 and Sr2 RhO4 are not only isoelectronic but also isostructural with a crystal structure similar to that of Sr2 RuO4 and La2 CuO4 .16 A unique and important structural feature shared by both Sr2 IrO4 and Sr2 RhO4 is that they crystallize in a reduced tetragonal structure with space-group I 41 /acd due to a rotation of the IrO6 or RhO6 octahedra ◦ ◦ about the c axis by ∼12 or , respectively, resulting in √ √ ∼9.7 16,19–21 a larger unit cell by 2 × 2 × 2, as compared to the undistorted cell. That the two isostructural and isoelectronic compounds exhibit the sharply contrasting physical properties underscores the critical role SOI plays in determining the ground state of the iridate. In this work, we tune the ground state via reducing SOI by substituting Rh4+ (4d 5 ) for Ir4+ (5d 5 ) in Sr2 IrO4, i.e., in single-crystal Sr2 Ir1−x Rhx O4 (0 x 1). As schematically illustrated in Fig. 1(a), the Rh substitution, unlike other chemical substitutions, directly reduces the SOI, thus the splitting between the Jeff = 1/2 and Jeff = 3/2 bands but without obviously altering the band ﬁlling. Hence, the system remains tuned at the Mott instability and is very susceptible to disorder scattering which gives rise to localization. For comparison and contrast, we also substitute Ru4+ (4d 4 ) for Ir4+ (5d 5 ) in Sr2 IrO4 , i.e., Sr2 Ir1−x Rux O4 (0 x 1), where Ru not only reduces the SOI but also ﬁlls the t2g bands with holes, which lowers EF , thus moving the system away from the Mott instability. Disorder scattering is then less relevant, and Ru doping systematically drives the system to a robust metallic state. The anticipated underlying effects of Ru doping on the Jeff = 1/2 and Jeff = 3/2 bands are also schematically illustrated in Fig. 1(a). The doping profoundly alters the

125105-1

©2012 American Physical Society

T. F. QI et al.

PHYSICAL REVIEW B 86, 125105 (2012)

However, the present work addresses structural and physical properties of bulk single-crystal Sr2 Ir1−x Rhx O4 with x ranging from 0 to 1. II. EXPERIMENTAL

FIG. 1. (Color online) (a) The schematics for the effects of Rh and Ru doping on the Jeff = 1/2 and Jeff = 3/2 bands; the Rh concentration x dependence at 90 K of (b) the lattice parameters’ a and c axes (right scale), and (c) the unit cell volume V and the Ir-O-Ir angle θ (right scale). (d) Some representative single-crystal Sr2 Ir1−x Rhx O4 and (e) their Bragg diffraction peaks ([100] and [001] directions); note the highly ordered crystal structure.

balance between the competing local energies; namely, the SOI is weakened, while the tetragonal CEF and the Hund’s coupling JH are increased. In addition, the Rh and Ir atoms are randomly distributed over the octahedra, hindering the hopping of the d electrons because of a mismatch of the energy levels and a mismatch of the rotation of the octahedra. The resulting disorder scattering gives rise to localized states. The combined effects produces a rich T-x phase diagram in Sr2 Ir1−x Rhx O4 featuring two major effects: (1) Light Rh doping (0 x 0.16) effectively reduces the SOI and prompts a simultaneous and precipitous drop in both the electrical resistivity ρ(T ) and the magnetic ordering temperature TC , which becomes zero at x = 0.16 from 240 K at x = 0. The results indicate that the Rh concentration does provide a degree of control on the splitting between Jeff = 1/2 and Jeff = 3/2 bands. (2) However, heavier Rh doping [0.24 < x < 0.85 (±0.05)] increases localization effects in the system which fosters a return to an insulating state with anomalous magnetic behavior occurring below 0.3 K that only disappears near x = 1. The magnetic state is expected to arise from the strong competition between antiferromagnetic (AFM) and ferromagnetic (FM) coupling that causes strong spin frustration. A recent optical study 26 on thin-ﬁlm Sr2 Ir1−x Rhx O4 with x up to 0.26 is qualitatively consistent with some of our results.

The single crystals studied were grown from offstoichiometric quantities of SrCl2 , SrCO3 , IrO2 , and RhO2 or RuO2 using self-ﬂux techniques. Similar technical details are described elsewhere.6,8–10 The size of the single crystals is as large as 1.0 × 1.0 × 0.2 cm3 [see Fig. 1(d)]. The structures of Sr2 Ir1−x Rhx O4 and Sr2 Ir1−x Rux O4 were determined using a Nonius Kappa CCD x-ray diffractometer at 90 K and 295 K. Structures were reﬁned by full-matrix least squares using the SHELX-97 programs.27 The standard deviations of all lattice parameters and interatomic distances are smaller than 0.1%. The structure of the single crystals studied is highly ordered, as evidenced by sharp and bright Bragg diffraction spots along the [100] and [001] directions, respectively, in Fig. 1(e). We also checked the atom site occupancy factor on oxygen sites by running a test in which the oxygen occupancies were allowed to reﬁne freely. They are all reﬁned with full-occupancy factors, suggesting that no clear oxygen vacancy was found from the reﬁnement. Chemical compositions of the single crystals were determined using a combined unit of Hitachi/Oxford SwiftED 3000 for energy dispersive x-ray (EDX) spectroscopy. The speciﬁc heat, C(T ), was measured down to 50 mK whereas the resistivity, ρ(T ), and the magnetization, M(T ), were measured between 1.7 K and 400 K using a Quantum Design (QD) 7T SQUID magnetometer and a QD 14T Physical Property Measurement System, respectively. III. RESULTS AND DISCUSSION

Substituting Rh4+ for Ir4+ results in a nearly uniform reduction in the lattice parameters’ a c axes and the unit cell V that is shrunk by ∼2%, as shown in Figs. 1(b) and 1(c). This behavior is expected for Rh4+ doping because the ionic radius ˚ is smaller than that of Ir4+ (0.625 A). ˚ [An of Rh4+ (0.600 A) increase in the lattice parameters would be anticipated instead for Rh3+ (4d 6 ) doping because of the larger ionic radius of ˚ The a axis is compressed by 0.87% whereas Rh3+ , 0.670 A.] the c axis only by 0.26%, which enhances the tetragonal CEF. In addition, the Ir-O-Ir bond angle θ increases signiﬁcantly near x = 0.16, indicating a less distorted lattice for x > 0.16. It is already established that θ is critical to the electronic and magnetic structure of Sr2 IrO4 .7–10,25 Rh doping effectively suppresses the magnetic transition TC from 240 K at x = 0 to zero at x = 0.16, as shown in Figs. 2(a), 2(b), and 2(c). With increasing x, the c-axis magnetization Mc becomes relatively stronger at μ0 H = 0.1 T. This is consistent with the reduced magnetic anisotropy in isothermal magnetization M(H ) for x = 0.11 at T = 1.7 K and near μ0 H = 1 T, as shown in the inset in Fig. 2(b); the ratio Ma /Mc at lower ﬁelds ( 0, and a largely reduced magnitude of ρ a (T ) ranging from 10−3 to 10−1 cm [see Fig. 3(b)]. dρ a /dT > 0 becomes most obvious at x = 0.11. The corresponding c-axis resistivity ρ c (T ) shows a slightly larger magnitude, but with dρ c /dT remaining negative, as

FIG. 2. (Color online) The temperature dependence at μ0 H = 0.1 T of the magnetization (a) Ma , (b) Mc for 0 x 0.15 and isothermal magnetization Ma and Mc for x = 0.11 at T = 1.7 K (inset); and (c) Ma for 0.24 x 0.75 and χa−1 (right scale) for x = 0, 0.42, and 0.70. (d) The Rh concentration x dependence of TC and θ CW , and the magnetic effective moment μeff (inset).

law χ = χ 0 + C/(T + θ CW ) for a temperature range of 50–350 K for x > 0.16 (χ 0 is a temperature-independent constant, θ CW the Curie-Weiss temperature, and C the Curie constant); and we then used χ 0 to obtain χ = C/(T + θ CW ) and plotted the data in terms of χ −1 vs T , as shown in Fig. 2(c) (right scale). θ CW tracks the rapidly decreasing TC for 0 x 0.16, and becomes nearly zero at x = 0.16 and then changes its sign from positive to negative as x further increases. It is remarkable that θ CW is −72 K at x = 0.42 and then becomes −2 K at x = 1, as shown in Fig. 2(d). Since θ CW measures the strength of the magnetic interaction, such a large absolute value of θ CW (= −72 K) in a system without magnetic ordering above 0.3 K (magnetic order below 0.3 K is observed and discussed below) implies a strong suppression of magnetic ordering or spin frustration. It becomes conceivable that both the disappearance of the magnetic order at x = 0.16 and the appearance of the spin frustration at higher x are a

FIG. 3. (Color online) The temperature dependence for Sr2 Ir1−x Rhx O4 of (a) the resistivity ρ for x = 0 and 0.07; (b) the a-axis resistivity ρ a for x = 0.11, 0.15, and 0.24; (c) ρ a for x = 0.42, 0.70, and 0.75; (d) the c-axis resistivity ρ c for x = 0.11 and 0.15; (e) ρ c for x = 0.42, 0.70, and 0.75. Inset in (a): The ratio of ρ(2 K)/ρ(300 K) vs x; inset in (c): ln ρ a vs T −1/2 ; inset in (d): ρ a vs T for Sr2 Ir1−x Rux O4 , where a robust metallic state occurs at x = 0.50.

125105-3

T. F. QI et al.

PHYSICAL REVIEW B 86, 125105 (2012)

shown in Fig. 3(d). Since the bond angle θ , which is critical to electron hopping in general, remains essentially unchanged until x > 0.16 [Fig. 1(c)] and the Rh doping adds no holes or electrons to the bands, the drastic reductions in ρ a (T ) and ρ c (T ) may be primarily due to the weakened SOI. In addition, the vanishing magnetic state in this doping range may also help reduce the band gap because the internal magnetic ﬁeld lifts the degeneracy along the edge of the AF Brillouin zone, thus facilitating the SOI to open a full gap in the presence of U .5 Both ρ a (T ) and ρ c (T ) exhibit a noticeable upturn below 50 K indicating that a low-temperature metallic state is not fully realized although ρ a (T ) and ρ c (T ) are radically reduced by six orders of magnitude. It is also noted that ρ a (T ) for x = 0.24 follows variable range hopping (VRH) model, ρ ∼ exp(1/T )1/2 , below 50 K. It implies that Anderson localization comes into play at x = 0.24. The persisting nonmetallic state below 50 K suggests that the band gap is not fully closed with conducting states despite the weakened SOI and the diminishing internal magnetic ﬁeld. It is interesting to see that 14% of Ru doping, which not only reduces SOI but also adds holes to the bands, also fails to induce a metallic state [see inset in Fig. 3(d)]. Region II, 0.24 < x < 0.85 (±0.05). If the reduction of SOI were the only mechanism, a more metallic state would be expected with increasing x. However, both ρ a (T ) and ρ c (T ) increase signiﬁcantly, reaching 105 and 107 cm, respectively, at low temperatures for x = 0.70 before dropping again to 10−1 cm for x = 0.75, as shown in Figs. 3(c) and 3(e). No metallic behavior (dρ/dT > 0) is observed in the entire temperature range measured for x = 0.42, 0.70, and 0.75. The insulating state occurring in this region is the consequence of localization due to disorder on the Rh/Ir site in the alloy. ρ for these Rh concentrations ﬁts the VRH ρ ∼ exp(1/T )1/2 for 2 < T < 100 K, suggesting that Anderson localization due to disorder becomes signiﬁcant in the presence of Coulomb interaction.28 However, it cannot be ruled out that there might exist clusters of Rh-doped areas although the single crystals studied are highly ordered [Fig. 1(e)]. It sharply contrasts the well-established metallic state in Sr2 Ir1−x Rux O4 with x = 0.50 [inset of Fig. 3(d)]. It is important to note that our oxygenated single crystals with x = 0.42, 0.70, and 0.75 exhibit essentially identical magnitude and temperature dependence of ρ a (T ) and ρ c (T ); this result rules out an insulating state that might be induced by oxygen deﬁciency. Indeed, the x-ray reﬁnement already conﬁrms no discernible oxygen deﬁciency in the single crystals studied. The ratio of ρ(2 K)/ρ (300 K) for both ρ a (T ) and ρ c (T ) qualitatively captures the change of transport properties with Rh concentration x [see inset in Fig. 3(c)]. The initial, precipitous drop in the ratio from ∼106 at x = 0 to ∼1 near x = 0.16 signals the rapidly growing metallic-like state. The ratio rises again at x > 0.24, marking the return to an insulating state, before falling back for x > 0.70. The effective moment μeff essentially tracks the change of the ratio of ρ(2 K)/ρ(300 K). This reﬂects the association of localized states with the magnetic degrees of freedom [inset in Fig. 2(d)]. The temperature dependence of the speciﬁc heat C for various x is shown in Fig. 4(a). Fitting the data to C(T ) = γ T + βT 3 for 10 < T < 50 K yields the coefﬁcient for the electronic contribution to C(T ), γ , that systematically

FIG. 4. (Color online) (a) The speciﬁc heat C(T )/T vs T 2 for Sr2 Ir1−x Rhx O4 ; (b) C(T )/T vs T for 50 mK < T < 20 K at μ0 H = 0 for x = 0.42 and 0.70, and 9 T for x = 0.42; (c) C(T )/T vs T 2 for Sr2 Ir1−x Rux O4 for comparison; (d) γ vs x for Sr2 Ir1−x Rhx O4 and Sr2 Ir1−x Rux O4 .

increases with x from 7 mJ/mole K2 at x = 0 to 30 mJ/mole K2 at x = 1. The increased γ for the insulating region 0.24 < x 0.75 may be a result of the states that are localized due to disorder in the gap, which give rise to a ﬁnite density of states [Fig. 4(d)]. Since Rh is not a dopant in the conventional sense, the conventional picture of hydrogen-like impurities does not apply. However, any breaking of the translational invariance of the system (such as Rh ions) necessarily introduces a bound state in the gap of the semiconductor. This leads to a gradual ﬁlling of the gap with x. Remarkably, C(T )/T exhibits a pronounced peak near TM = 100 mK and 280 mK for x = 0.42 and 0.70, respectively, which can be completely suppressed by a magnetic ﬁeld H of 9 T [Fig. 4(b)]. This anomaly signals a transition to a low-T spin order from a higher-T spin frustration characterized by a frustration parameter f = |θCW |/TM = |−72|/0.1 = 720 for

125105-4

SPIN-ORBIT TUNED METAL-INSULATOR TRANSITIONS . . .

FIG. 5. (Color online) The phase diagram for Sr2 Ir1−x Rhx O4 generated based on the data presented above. Note that PM stands for paramagnetic and NMS nonmetallic state.

x = 0.42, for example. In contrast, Sr2 Ir1−x Rux O4 behaves more normally [Fig. 4(c)], yielding γ considerably larger than that for Sr2 Ir1−x Rhx O4 [Fig. 4(d)], which is consistent with the robust metallic state. Figure 5 shows a phase diagram for Sr2 Ir1−x Rhx O4 generated based on the data presented above which summarizes the central ﬁndings of this study. The initial Rh doping effectively reduces the SOI, or the splitting between the Jeff = 1/2 and Jeff = 3/2 bands, and alters the relative strength of the SOI and the tetragonal CEF that dictates the magnetic state, which, in turn, affects the band gap near EF . In addition, the Rh doping also enhances the Hund’s rule coupling that competes with the SOI, and prevents the formation of the Jeff = 1/2 state.5 It is these SOI-induced changes that account for the simultaneous, precipitate decrease in ρ(T ) and TC that vanishes at x = 0.16. As x increases further, the Rh/Ir disorder on the transition-metal site determines the properties of the

*

High school student on internship, Paul Lawrence Dunber High School, Lexington, Kentucky 40513, USA. † Corresponding author: [email protected] 1 B. J. Kim, Hosub Jin, S. J. Moon, J.-Y. Kim, B.-G. Park, C. S. Leem, Jaejun Yu, T. W. Noh, C. Kim, S.-J. Oh, V. Durairai, G. Cao, and J.-H. Park, Phys. Rev. Lett. 101, 076402 (2008). 2 S. J. Moon, H. Jin, K. W. Kim, W. S. Choi, Y. S. Lee, J. Yu, G. Cao, A. Sumi, H. Funakubo, C. Bernhard, and T. W. Noh, Phys. Rev. Lett. 101, 226401 (2008). 3 B. J. Kim, H. Ohsumi, T. Komesu, S. Sakai, T. Morita, H. Takagi, and T. Arima, Science 323, 1329 (2009). 4 D. Haskel, G. Fabbris, Mikhail Zhernenkov, P. P. Kong, C. Jin, G. Cao, and M. van Veenendaal, Phys. Rev. Lett. 109, 027204 (2012). 5 Hiroshi Watanabe, Tomonori Shirakawa, and Seiji Yunoki, Phys. Rev. Lett. 105, 216410 (2010). 6 G. Cao, J. Bolivar, S. McCall, J. E. Crow, and R. P. Guertin, Phys. Rev. B 57, R11039 (1998). 7 G. Jackeli and G. Khaliulin, Phys. Rev. Lett. 102, 017205 (2009). 8 S. Chikara, O. Korneta, W. P. Crummett, L. E. DeLong, P. Schlottmann, and G. Cao, Phys. Rev. B 80, 140407 (R) (2009).

PHYSICAL REVIEW B 86, 125105 (2012)

system. There is an energy level mismatch for the Rh and Ir sites that makes the hopping of the carriers between an octahedron containing a Rh atom and one with an Ir ion more difﬁcult and also changes the orientation angles of the octahedra. The randomness of the Rh/Ir occupations gives rise to Anderson localization and an insulating state for 0.24 < x < 0.85 (±0.05). In addition, the SOI may no longer be strong enough to support the Jeff = 1/2 insulating state and the Hund’s rule coupling is enhanced (on the Rh sites), hence further strengthening the competition between AFM and FM couplings. As a result of this competition, spin frustration arises at intermediate temperatures. The occurrence of a spinordered state below 0.3 K along with the high θ CW corroborates the frustrated state. These effects diminish with disappearing disorder when x approaches 1, where the weakened SOI is comparable to other relevant energies yielding a metallic state. This point is qualitatively consistent with the recent theoretical studies for Sr2 RhO4 .15,20,21 In contrast, there is no discernible effect due to disorder in Sr2 Ir1−x Rux O4 . While for isoelectronic Rh substitution the system always remains in the proximity to the Mott condition for an insulator, each Ru atom adds one hole, giving rise to a higher density of states near EF and hence supporting a more robust metallic state in Sr2 RuO4 . Under these circumstances disorder in the alloy plays a less relevant role. ACKNOWLEDGMENTS

G.C. is very grateful to G. Khaliulin, X. Dai, Y. B. Kim, H. Y. Kee, and G. Jackeli for enlightening discussions. This work was supported by the NSF through Grants No. DMR0856234 (G.C.), No. EPS-0814194 (G.C., R.K.K.), and No. DMR-1056536 (R.K.K.) and by the Department of Energy through Grant No. DE-FG02-98ER45707 (P.S.).

9

O. B. Korneta, Tongfei Qi, S. Chikara, S. Parkin, L. E. DeLong, P. Schlottmann, and G. Cao, Phys. Rev. B 82, 115117 (2010). 10 M. Ge, T. F. Qi, O. B. Korneta, L. E. De Long, P. Schlottmann, and G. Cao, Phys. Rev. B 84, 100402(R) (2011). 11 I. Franke, P. J. Baker, S. J. Blundell, T. Lancaster, W. Hayes, F. L. Pratt, and G. Cao, Phys. Rev. B 83, 094416 (2011). 12 Fa Wang and T. Senthil, Phys. Rev. Lett. 106, 136402 (2011). 13 D. Hsieh, F. Mahmood, D. Torchinsky, G. Cao, and N. Gedik, Phys. Rev. B 86, 035128 (2012). 14 Q. Wang, Y. Cao, J. A. Waugh, T. F. Qi, O. B. Korneta, G. Cao, and D. S. Dessau (unpublished). 15 Cyril Martins, Markus Aichhorn, Loig Vaugier, and Silke Biermann, Phys. Rev. Lett. 107, 266404 (2011). 16 M. A. Subramanian, M. K. Crawford, R. L. Harlow, T. Ami, J. A. Fernandez-Baca, Z. R. Wang, and D. C. Johnston, Physica C 235, 743 (1994). 17 R. S. Perry, F. Baumberger, L. Balicas, N. Kikugawa, N. J. Ingle, A. Rost, J. F. Mercure, Y. Maeno, Z. X. Shen, and A. P. Mackenzie, New J. Phys. 8, 175 (2006).

125105-5

T. F. QI et al. 18

PHYSICAL REVIEW B 86, 125105 (2012)

S. J. Moon, M. W. Kim, K. W. Kim, Y. S. Lee, J.-Y. Kim, J.-H. Park, B. J. Kim, S.-J. Oh, S. Nakatsuji, Y. Maeno, I. Nagai, S. I. Ikeda, G. Cao, and T. W. Noh, Phys. Rev. B 74, 113104 (2006). 19 Q. Huang, J. L. Soubeyroux, O. Chmaissen, I. Natali Sora, A. Santoro, R. J. Cava, J. J. Krajewski, and W. F. Peck, Jr., J. Solid State Chem. 112, 355 (1994). 20 R. J. Cava, B. Batlogg, K. Kiyono, H. Takagi, J. J. Krajewski, W. F. Peck, Jr., L. W. Rupp, Jr., and C. H. Chen, Phys. Rev. B 49, 11890 (1994). 21 M. K. Crawford, M. A. Subramanian, R. L. Harlow, J. A. FernandezBaca, Z. R. Wang, and D. C. Johnston, Phys. Rev. B 49, 9198 (1994).

22

Y. Maeno, H. Hashimoto, K. Yoshida, S. Nishizaki, T. Fujita, J. G. Bednorz, and F. Lichtenberg, Nature (London) 372, 532 (1994). 23 M. W. Haverkort, I. S. Elﬁmov, L. H. Tjeng, G. A. Sawatzky, and A. Damascelli, Phys. Rev. Lett. 101, 026406 (2008). 24 Guo-Qiang Liu, V. N. Antonov, O. Jepsen, and O. K. Andersen, Phys. Rev. Lett. 101, 26408 (2008). 25 S. J. Moon, Hosub Jin, W. S. Choi, J. S. Lee, S. S. A. Seo, J. Yu, G. Cao, T. W. Noh, and Y. S. Lee, Phys. Rev. B 80, 195110 (2009). 26 J. S. Lee, Y. Krockenberger, K. S. Takahashi, M. Kawasaki, and Y. Tokura, Phys. Rev. B 85, 035101 (2012). 27 G. M. Sheldrick, Acta Crystallogr. Sect. A 64, 112 (2008). 28 Nevill Mott, Metal-Insulator Transition (Taylor & Francis, London, 1990), p. 52.

125105-6

Spin-orbit tuned metal-insulator transitions in single-crystal Sr2 Ir1−x Rh x O4 (0 x 1) T. F. Qi,1 O. B. Korneta,1 L. Li,1 K. Butrouna,1 V. S. Cao,1,* Xiangang Wan,2 P. Schlottmann,3 R. K. Kaul,1 and G. Cao1,† 1

Center for Advanced Materials and Department of Physics and Astronomy, University of Kentucky, Lexington, Kentucky 40506, USA 2 Department of Physics, Nanjing University, Nanjing, People’s Republic of China 3 Department of Physics, Florida State University, Tallahassee, Florida 32306, USA (Received 28 June 2012; revised manuscript received 8 August 2012; published 6 September 2012) Sr2 IrO4 is a magnetic insulator driven by spin-orbit interaction (SOI) whereas the isoelectronic and isostructural Sr2 RhO4 is a paramagnetic metal. The contrasting ground states have been shown to result from the critical role of the strong SOI in the iridate. Our investigation of structural, transport, magnetic, and thermal properties reveals that substituting 4d Rh4+ (4d 5 ) ions for 5d Ir4+ (5d 5 ) ions in Sr2 IrO4 directly reduces the SOI and rebalances the competing energies so profoundly that it generates a rich phase diagram for Sr2 Ir1−x Rhx O4 featuring two major effects: (1) Light Rh doping (0 x 0.16) prompts a simultaneous and precipitous drop in both the electrical resistivity and the magnetic ordering temperature TC , which is suppressed to zero at x = 0.16 from 240 K at x = 0. (2) However, with heavier Rh doping [0.24 < x < 0.85 (±0.05)] disorder scattering leads to localized states and a return to an insulating state with spin frustration and exotic magnetic behavior that only disappears near x = 1. The intricacy of Sr2 Ir1−x Rhx O4 is further highlighted by comparison with Sr2 Ir1−x Rux O4 where Ru4+ (4d 4 ) drives a direct crossover from the insulating to metallic states. DOI: 10.1103/PhysRevB.86.125105

PACS number(s): 75.70.Tj, 71.30.+h

I. INTRODUCTION

Sr2 IrO4 is an archetype for new physics primarily driven by the interplay of electron-electron and spin-orbit interactions (SOI).1–3 The relativistic SOI proportional to Z 4 (Z is the atomic number) is approximately 0.4 eV in the iridate (compared to ∼20 meV in 3d materials), and splits the t2g bands into bands with Jeff = 1/2 and Jeff = 3/2, the latter having lower energy.1,2 Since the Ir4+ (5d 5 ) ions provide ﬁve 5d electrons, four of them ﬁll the lower Jeff = 3/2 bands, and one electron partially ﬁlls the Jeff = 1/2 band where the Fermi level EF resides. The Jeff = 1/2 band is so narrow that even a reduced on-site Coulomb repulsion U (∼0.5 eV) due to the extended nature of 5d-electron orbitals is sufﬁcient to open a small gap (0.1 eV) supporting the insulating state.1,2 Most recently, an x-ray absorption spectroscopy study indicates a mixing of the Jeff = 1/2 and Jeff = 3/2 bands as a result of exchange interactions (∼0.2 eV) and a tetragonal crystal electric ﬁeld (CEF) (∼0.075 eV).4 Nevertheless, the larger the SOI and the narrower the band is, the smaller U is needed for a SOI-related insulating state,5 in which SOI, Coulomb interactions, tetragonal CEF, and Hund’s coupling JH become so comparable that they vigorously compete with each other, setting a new balance between the relevant energies that can drive new exotic states.1–18 In contrast, the isoelectronic 4d-based Sr2 RhO4 with Rh4+ (4d 5 ) ions with ﬁve 4d electrons has a weaker SOI (∼0.16 eV), thus a smaller splitting between the Jeff = 1/2 and Jeff = 3/2 bands that are more evenly ﬁlled by the ﬁve 4d electrons.5,15–18 The weaker SOI combined with more effectively screened Coulomb interactions between O 2p and Rh 4d electrons favors a metallic state.15 Indeed, Sr2 RhO4 is a paramagnetic, correlated metal16–18 sharply contrasting the magnetic insulator Sr2 IrO4 that orders at TC = 240 K.6,19–21 In addition, comparisons of Sr2 RhO4 with another 4d-based compound, Sr2 RuO4 , a p-wave superconductor, 22 reveal that the impact of the SOI strongly depends on the detailed band structure near the Fermi surface EF , the Coulomb interactions, 1098-0121/2012/86(12)/125105(6)

and the lattice distortions.7,15,23,24 The t2g bands in Sr2 RhO4 near EF are less dispersive than those in Sr2 RuO4 , therefore more susceptible to the SOI-induced band shifts near EF than in Sr2 RuO4 despite the similar strength of the SOI in both materials.23 This is in part because the Ru4+ (4d 4 ) ion has four 4d electrons instead of ﬁve; Ru doping therefore adds holes to the bands. Both Sr2 IrO4 and Sr2 RhO4 are not only isoelectronic but also isostructural with a crystal structure similar to that of Sr2 RuO4 and La2 CuO4 .16 A unique and important structural feature shared by both Sr2 IrO4 and Sr2 RhO4 is that they crystallize in a reduced tetragonal structure with space-group I 41 /acd due to a rotation of the IrO6 or RhO6 octahedra ◦ ◦ about the c axis by ∼12 or , respectively, resulting in √ √ ∼9.7 16,19–21 a larger unit cell by 2 × 2 × 2, as compared to the undistorted cell. That the two isostructural and isoelectronic compounds exhibit the sharply contrasting physical properties underscores the critical role SOI plays in determining the ground state of the iridate. In this work, we tune the ground state via reducing SOI by substituting Rh4+ (4d 5 ) for Ir4+ (5d 5 ) in Sr2 IrO4, i.e., in single-crystal Sr2 Ir1−x Rhx O4 (0 x 1). As schematically illustrated in Fig. 1(a), the Rh substitution, unlike other chemical substitutions, directly reduces the SOI, thus the splitting between the Jeff = 1/2 and Jeff = 3/2 bands but without obviously altering the band ﬁlling. Hence, the system remains tuned at the Mott instability and is very susceptible to disorder scattering which gives rise to localization. For comparison and contrast, we also substitute Ru4+ (4d 4 ) for Ir4+ (5d 5 ) in Sr2 IrO4 , i.e., Sr2 Ir1−x Rux O4 (0 x 1), where Ru not only reduces the SOI but also ﬁlls the t2g bands with holes, which lowers EF , thus moving the system away from the Mott instability. Disorder scattering is then less relevant, and Ru doping systematically drives the system to a robust metallic state. The anticipated underlying effects of Ru doping on the Jeff = 1/2 and Jeff = 3/2 bands are also schematically illustrated in Fig. 1(a). The doping profoundly alters the

125105-1

©2012 American Physical Society

T. F. QI et al.

PHYSICAL REVIEW B 86, 125105 (2012)

However, the present work addresses structural and physical properties of bulk single-crystal Sr2 Ir1−x Rhx O4 with x ranging from 0 to 1. II. EXPERIMENTAL

FIG. 1. (Color online) (a) The schematics for the effects of Rh and Ru doping on the Jeff = 1/2 and Jeff = 3/2 bands; the Rh concentration x dependence at 90 K of (b) the lattice parameters’ a and c axes (right scale), and (c) the unit cell volume V and the Ir-O-Ir angle θ (right scale). (d) Some representative single-crystal Sr2 Ir1−x Rhx O4 and (e) their Bragg diffraction peaks ([100] and [001] directions); note the highly ordered crystal structure.

balance between the competing local energies; namely, the SOI is weakened, while the tetragonal CEF and the Hund’s coupling JH are increased. In addition, the Rh and Ir atoms are randomly distributed over the octahedra, hindering the hopping of the d electrons because of a mismatch of the energy levels and a mismatch of the rotation of the octahedra. The resulting disorder scattering gives rise to localized states. The combined effects produces a rich T-x phase diagram in Sr2 Ir1−x Rhx O4 featuring two major effects: (1) Light Rh doping (0 x 0.16) effectively reduces the SOI and prompts a simultaneous and precipitous drop in both the electrical resistivity ρ(T ) and the magnetic ordering temperature TC , which becomes zero at x = 0.16 from 240 K at x = 0. The results indicate that the Rh concentration does provide a degree of control on the splitting between Jeff = 1/2 and Jeff = 3/2 bands. (2) However, heavier Rh doping [0.24 < x < 0.85 (±0.05)] increases localization effects in the system which fosters a return to an insulating state with anomalous magnetic behavior occurring below 0.3 K that only disappears near x = 1. The magnetic state is expected to arise from the strong competition between antiferromagnetic (AFM) and ferromagnetic (FM) coupling that causes strong spin frustration. A recent optical study 26 on thin-ﬁlm Sr2 Ir1−x Rhx O4 with x up to 0.26 is qualitatively consistent with some of our results.

The single crystals studied were grown from offstoichiometric quantities of SrCl2 , SrCO3 , IrO2 , and RhO2 or RuO2 using self-ﬂux techniques. Similar technical details are described elsewhere.6,8–10 The size of the single crystals is as large as 1.0 × 1.0 × 0.2 cm3 [see Fig. 1(d)]. The structures of Sr2 Ir1−x Rhx O4 and Sr2 Ir1−x Rux O4 were determined using a Nonius Kappa CCD x-ray diffractometer at 90 K and 295 K. Structures were reﬁned by full-matrix least squares using the SHELX-97 programs.27 The standard deviations of all lattice parameters and interatomic distances are smaller than 0.1%. The structure of the single crystals studied is highly ordered, as evidenced by sharp and bright Bragg diffraction spots along the [100] and [001] directions, respectively, in Fig. 1(e). We also checked the atom site occupancy factor on oxygen sites by running a test in which the oxygen occupancies were allowed to reﬁne freely. They are all reﬁned with full-occupancy factors, suggesting that no clear oxygen vacancy was found from the reﬁnement. Chemical compositions of the single crystals were determined using a combined unit of Hitachi/Oxford SwiftED 3000 for energy dispersive x-ray (EDX) spectroscopy. The speciﬁc heat, C(T ), was measured down to 50 mK whereas the resistivity, ρ(T ), and the magnetization, M(T ), were measured between 1.7 K and 400 K using a Quantum Design (QD) 7T SQUID magnetometer and a QD 14T Physical Property Measurement System, respectively. III. RESULTS AND DISCUSSION

Substituting Rh4+ for Ir4+ results in a nearly uniform reduction in the lattice parameters’ a c axes and the unit cell V that is shrunk by ∼2%, as shown in Figs. 1(b) and 1(c). This behavior is expected for Rh4+ doping because the ionic radius ˚ is smaller than that of Ir4+ (0.625 A). ˚ [An of Rh4+ (0.600 A) increase in the lattice parameters would be anticipated instead for Rh3+ (4d 6 ) doping because of the larger ionic radius of ˚ The a axis is compressed by 0.87% whereas Rh3+ , 0.670 A.] the c axis only by 0.26%, which enhances the tetragonal CEF. In addition, the Ir-O-Ir bond angle θ increases signiﬁcantly near x = 0.16, indicating a less distorted lattice for x > 0.16. It is already established that θ is critical to the electronic and magnetic structure of Sr2 IrO4 .7–10,25 Rh doping effectively suppresses the magnetic transition TC from 240 K at x = 0 to zero at x = 0.16, as shown in Figs. 2(a), 2(b), and 2(c). With increasing x, the c-axis magnetization Mc becomes relatively stronger at μ0 H = 0.1 T. This is consistent with the reduced magnetic anisotropy in isothermal magnetization M(H ) for x = 0.11 at T = 1.7 K and near μ0 H = 1 T, as shown in the inset in Fig. 2(b); the ratio Ma /Mc at lower ﬁelds ( 0, and a largely reduced magnitude of ρ a (T ) ranging from 10−3 to 10−1 cm [see Fig. 3(b)]. dρ a /dT > 0 becomes most obvious at x = 0.11. The corresponding c-axis resistivity ρ c (T ) shows a slightly larger magnitude, but with dρ c /dT remaining negative, as

FIG. 2. (Color online) The temperature dependence at μ0 H = 0.1 T of the magnetization (a) Ma , (b) Mc for 0 x 0.15 and isothermal magnetization Ma and Mc for x = 0.11 at T = 1.7 K (inset); and (c) Ma for 0.24 x 0.75 and χa−1 (right scale) for x = 0, 0.42, and 0.70. (d) The Rh concentration x dependence of TC and θ CW , and the magnetic effective moment μeff (inset).

law χ = χ 0 + C/(T + θ CW ) for a temperature range of 50–350 K for x > 0.16 (χ 0 is a temperature-independent constant, θ CW the Curie-Weiss temperature, and C the Curie constant); and we then used χ 0 to obtain χ = C/(T + θ CW ) and plotted the data in terms of χ −1 vs T , as shown in Fig. 2(c) (right scale). θ CW tracks the rapidly decreasing TC for 0 x 0.16, and becomes nearly zero at x = 0.16 and then changes its sign from positive to negative as x further increases. It is remarkable that θ CW is −72 K at x = 0.42 and then becomes −2 K at x = 1, as shown in Fig. 2(d). Since θ CW measures the strength of the magnetic interaction, such a large absolute value of θ CW (= −72 K) in a system without magnetic ordering above 0.3 K (magnetic order below 0.3 K is observed and discussed below) implies a strong suppression of magnetic ordering or spin frustration. It becomes conceivable that both the disappearance of the magnetic order at x = 0.16 and the appearance of the spin frustration at higher x are a

FIG. 3. (Color online) The temperature dependence for Sr2 Ir1−x Rhx O4 of (a) the resistivity ρ for x = 0 and 0.07; (b) the a-axis resistivity ρ a for x = 0.11, 0.15, and 0.24; (c) ρ a for x = 0.42, 0.70, and 0.75; (d) the c-axis resistivity ρ c for x = 0.11 and 0.15; (e) ρ c for x = 0.42, 0.70, and 0.75. Inset in (a): The ratio of ρ(2 K)/ρ(300 K) vs x; inset in (c): ln ρ a vs T −1/2 ; inset in (d): ρ a vs T for Sr2 Ir1−x Rux O4 , where a robust metallic state occurs at x = 0.50.

125105-3

T. F. QI et al.

PHYSICAL REVIEW B 86, 125105 (2012)

shown in Fig. 3(d). Since the bond angle θ , which is critical to electron hopping in general, remains essentially unchanged until x > 0.16 [Fig. 1(c)] and the Rh doping adds no holes or electrons to the bands, the drastic reductions in ρ a (T ) and ρ c (T ) may be primarily due to the weakened SOI. In addition, the vanishing magnetic state in this doping range may also help reduce the band gap because the internal magnetic ﬁeld lifts the degeneracy along the edge of the AF Brillouin zone, thus facilitating the SOI to open a full gap in the presence of U .5 Both ρ a (T ) and ρ c (T ) exhibit a noticeable upturn below 50 K indicating that a low-temperature metallic state is not fully realized although ρ a (T ) and ρ c (T ) are radically reduced by six orders of magnitude. It is also noted that ρ a (T ) for x = 0.24 follows variable range hopping (VRH) model, ρ ∼ exp(1/T )1/2 , below 50 K. It implies that Anderson localization comes into play at x = 0.24. The persisting nonmetallic state below 50 K suggests that the band gap is not fully closed with conducting states despite the weakened SOI and the diminishing internal magnetic ﬁeld. It is interesting to see that 14% of Ru doping, which not only reduces SOI but also adds holes to the bands, also fails to induce a metallic state [see inset in Fig. 3(d)]. Region II, 0.24 < x < 0.85 (±0.05). If the reduction of SOI were the only mechanism, a more metallic state would be expected with increasing x. However, both ρ a (T ) and ρ c (T ) increase signiﬁcantly, reaching 105 and 107 cm, respectively, at low temperatures for x = 0.70 before dropping again to 10−1 cm for x = 0.75, as shown in Figs. 3(c) and 3(e). No metallic behavior (dρ/dT > 0) is observed in the entire temperature range measured for x = 0.42, 0.70, and 0.75. The insulating state occurring in this region is the consequence of localization due to disorder on the Rh/Ir site in the alloy. ρ for these Rh concentrations ﬁts the VRH ρ ∼ exp(1/T )1/2 for 2 < T < 100 K, suggesting that Anderson localization due to disorder becomes signiﬁcant in the presence of Coulomb interaction.28 However, it cannot be ruled out that there might exist clusters of Rh-doped areas although the single crystals studied are highly ordered [Fig. 1(e)]. It sharply contrasts the well-established metallic state in Sr2 Ir1−x Rux O4 with x = 0.50 [inset of Fig. 3(d)]. It is important to note that our oxygenated single crystals with x = 0.42, 0.70, and 0.75 exhibit essentially identical magnitude and temperature dependence of ρ a (T ) and ρ c (T ); this result rules out an insulating state that might be induced by oxygen deﬁciency. Indeed, the x-ray reﬁnement already conﬁrms no discernible oxygen deﬁciency in the single crystals studied. The ratio of ρ(2 K)/ρ (300 K) for both ρ a (T ) and ρ c (T ) qualitatively captures the change of transport properties with Rh concentration x [see inset in Fig. 3(c)]. The initial, precipitous drop in the ratio from ∼106 at x = 0 to ∼1 near x = 0.16 signals the rapidly growing metallic-like state. The ratio rises again at x > 0.24, marking the return to an insulating state, before falling back for x > 0.70. The effective moment μeff essentially tracks the change of the ratio of ρ(2 K)/ρ(300 K). This reﬂects the association of localized states with the magnetic degrees of freedom [inset in Fig. 2(d)]. The temperature dependence of the speciﬁc heat C for various x is shown in Fig. 4(a). Fitting the data to C(T ) = γ T + βT 3 for 10 < T < 50 K yields the coefﬁcient for the electronic contribution to C(T ), γ , that systematically

FIG. 4. (Color online) (a) The speciﬁc heat C(T )/T vs T 2 for Sr2 Ir1−x Rhx O4 ; (b) C(T )/T vs T for 50 mK < T < 20 K at μ0 H = 0 for x = 0.42 and 0.70, and 9 T for x = 0.42; (c) C(T )/T vs T 2 for Sr2 Ir1−x Rux O4 for comparison; (d) γ vs x for Sr2 Ir1−x Rhx O4 and Sr2 Ir1−x Rux O4 .

increases with x from 7 mJ/mole K2 at x = 0 to 30 mJ/mole K2 at x = 1. The increased γ for the insulating region 0.24 < x 0.75 may be a result of the states that are localized due to disorder in the gap, which give rise to a ﬁnite density of states [Fig. 4(d)]. Since Rh is not a dopant in the conventional sense, the conventional picture of hydrogen-like impurities does not apply. However, any breaking of the translational invariance of the system (such as Rh ions) necessarily introduces a bound state in the gap of the semiconductor. This leads to a gradual ﬁlling of the gap with x. Remarkably, C(T )/T exhibits a pronounced peak near TM = 100 mK and 280 mK for x = 0.42 and 0.70, respectively, which can be completely suppressed by a magnetic ﬁeld H of 9 T [Fig. 4(b)]. This anomaly signals a transition to a low-T spin order from a higher-T spin frustration characterized by a frustration parameter f = |θCW |/TM = |−72|/0.1 = 720 for

125105-4

SPIN-ORBIT TUNED METAL-INSULATOR TRANSITIONS . . .

FIG. 5. (Color online) The phase diagram for Sr2 Ir1−x Rhx O4 generated based on the data presented above. Note that PM stands for paramagnetic and NMS nonmetallic state.

x = 0.42, for example. In contrast, Sr2 Ir1−x Rux O4 behaves more normally [Fig. 4(c)], yielding γ considerably larger than that for Sr2 Ir1−x Rhx O4 [Fig. 4(d)], which is consistent with the robust metallic state. Figure 5 shows a phase diagram for Sr2 Ir1−x Rhx O4 generated based on the data presented above which summarizes the central ﬁndings of this study. The initial Rh doping effectively reduces the SOI, or the splitting between the Jeff = 1/2 and Jeff = 3/2 bands, and alters the relative strength of the SOI and the tetragonal CEF that dictates the magnetic state, which, in turn, affects the band gap near EF . In addition, the Rh doping also enhances the Hund’s rule coupling that competes with the SOI, and prevents the formation of the Jeff = 1/2 state.5 It is these SOI-induced changes that account for the simultaneous, precipitate decrease in ρ(T ) and TC that vanishes at x = 0.16. As x increases further, the Rh/Ir disorder on the transition-metal site determines the properties of the

*

High school student on internship, Paul Lawrence Dunber High School, Lexington, Kentucky 40513, USA. † Corresponding author: [email protected] 1 B. J. Kim, Hosub Jin, S. J. Moon, J.-Y. Kim, B.-G. Park, C. S. Leem, Jaejun Yu, T. W. Noh, C. Kim, S.-J. Oh, V. Durairai, G. Cao, and J.-H. Park, Phys. Rev. Lett. 101, 076402 (2008). 2 S. J. Moon, H. Jin, K. W. Kim, W. S. Choi, Y. S. Lee, J. Yu, G. Cao, A. Sumi, H. Funakubo, C. Bernhard, and T. W. Noh, Phys. Rev. Lett. 101, 226401 (2008). 3 B. J. Kim, H. Ohsumi, T. Komesu, S. Sakai, T. Morita, H. Takagi, and T. Arima, Science 323, 1329 (2009). 4 D. Haskel, G. Fabbris, Mikhail Zhernenkov, P. P. Kong, C. Jin, G. Cao, and M. van Veenendaal, Phys. Rev. Lett. 109, 027204 (2012). 5 Hiroshi Watanabe, Tomonori Shirakawa, and Seiji Yunoki, Phys. Rev. Lett. 105, 216410 (2010). 6 G. Cao, J. Bolivar, S. McCall, J. E. Crow, and R. P. Guertin, Phys. Rev. B 57, R11039 (1998). 7 G. Jackeli and G. Khaliulin, Phys. Rev. Lett. 102, 017205 (2009). 8 S. Chikara, O. Korneta, W. P. Crummett, L. E. DeLong, P. Schlottmann, and G. Cao, Phys. Rev. B 80, 140407 (R) (2009).

PHYSICAL REVIEW B 86, 125105 (2012)

system. There is an energy level mismatch for the Rh and Ir sites that makes the hopping of the carriers between an octahedron containing a Rh atom and one with an Ir ion more difﬁcult and also changes the orientation angles of the octahedra. The randomness of the Rh/Ir occupations gives rise to Anderson localization and an insulating state for 0.24 < x < 0.85 (±0.05). In addition, the SOI may no longer be strong enough to support the Jeff = 1/2 insulating state and the Hund’s rule coupling is enhanced (on the Rh sites), hence further strengthening the competition between AFM and FM couplings. As a result of this competition, spin frustration arises at intermediate temperatures. The occurrence of a spinordered state below 0.3 K along with the high θ CW corroborates the frustrated state. These effects diminish with disappearing disorder when x approaches 1, where the weakened SOI is comparable to other relevant energies yielding a metallic state. This point is qualitatively consistent with the recent theoretical studies for Sr2 RhO4 .15,20,21 In contrast, there is no discernible effect due to disorder in Sr2 Ir1−x Rux O4 . While for isoelectronic Rh substitution the system always remains in the proximity to the Mott condition for an insulator, each Ru atom adds one hole, giving rise to a higher density of states near EF and hence supporting a more robust metallic state in Sr2 RuO4 . Under these circumstances disorder in the alloy plays a less relevant role. ACKNOWLEDGMENTS

G.C. is very grateful to G. Khaliulin, X. Dai, Y. B. Kim, H. Y. Kee, and G. Jackeli for enlightening discussions. This work was supported by the NSF through Grants No. DMR0856234 (G.C.), No. EPS-0814194 (G.C., R.K.K.), and No. DMR-1056536 (R.K.K.) and by the Department of Energy through Grant No. DE-FG02-98ER45707 (P.S.).

9

O. B. Korneta, Tongfei Qi, S. Chikara, S. Parkin, L. E. DeLong, P. Schlottmann, and G. Cao, Phys. Rev. B 82, 115117 (2010). 10 M. Ge, T. F. Qi, O. B. Korneta, L. E. De Long, P. Schlottmann, and G. Cao, Phys. Rev. B 84, 100402(R) (2011). 11 I. Franke, P. J. Baker, S. J. Blundell, T. Lancaster, W. Hayes, F. L. Pratt, and G. Cao, Phys. Rev. B 83, 094416 (2011). 12 Fa Wang and T. Senthil, Phys. Rev. Lett. 106, 136402 (2011). 13 D. Hsieh, F. Mahmood, D. Torchinsky, G. Cao, and N. Gedik, Phys. Rev. B 86, 035128 (2012). 14 Q. Wang, Y. Cao, J. A. Waugh, T. F. Qi, O. B. Korneta, G. Cao, and D. S. Dessau (unpublished). 15 Cyril Martins, Markus Aichhorn, Loig Vaugier, and Silke Biermann, Phys. Rev. Lett. 107, 266404 (2011). 16 M. A. Subramanian, M. K. Crawford, R. L. Harlow, T. Ami, J. A. Fernandez-Baca, Z. R. Wang, and D. C. Johnston, Physica C 235, 743 (1994). 17 R. S. Perry, F. Baumberger, L. Balicas, N. Kikugawa, N. J. Ingle, A. Rost, J. F. Mercure, Y. Maeno, Z. X. Shen, and A. P. Mackenzie, New J. Phys. 8, 175 (2006).

125105-5

T. F. QI et al. 18

PHYSICAL REVIEW B 86, 125105 (2012)

S. J. Moon, M. W. Kim, K. W. Kim, Y. S. Lee, J.-Y. Kim, J.-H. Park, B. J. Kim, S.-J. Oh, S. Nakatsuji, Y. Maeno, I. Nagai, S. I. Ikeda, G. Cao, and T. W. Noh, Phys. Rev. B 74, 113104 (2006). 19 Q. Huang, J. L. Soubeyroux, O. Chmaissen, I. Natali Sora, A. Santoro, R. J. Cava, J. J. Krajewski, and W. F. Peck, Jr., J. Solid State Chem. 112, 355 (1994). 20 R. J. Cava, B. Batlogg, K. Kiyono, H. Takagi, J. J. Krajewski, W. F. Peck, Jr., L. W. Rupp, Jr., and C. H. Chen, Phys. Rev. B 49, 11890 (1994). 21 M. K. Crawford, M. A. Subramanian, R. L. Harlow, J. A. FernandezBaca, Z. R. Wang, and D. C. Johnston, Phys. Rev. B 49, 9198 (1994).

22

Y. Maeno, H. Hashimoto, K. Yoshida, S. Nishizaki, T. Fujita, J. G. Bednorz, and F. Lichtenberg, Nature (London) 372, 532 (1994). 23 M. W. Haverkort, I. S. Elﬁmov, L. H. Tjeng, G. A. Sawatzky, and A. Damascelli, Phys. Rev. Lett. 101, 026406 (2008). 24 Guo-Qiang Liu, V. N. Antonov, O. Jepsen, and O. K. Andersen, Phys. Rev. Lett. 101, 26408 (2008). 25 S. J. Moon, Hosub Jin, W. S. Choi, J. S. Lee, S. S. A. Seo, J. Yu, G. Cao, T. W. Noh, and Y. S. Lee, Phys. Rev. B 80, 195110 (2009). 26 J. S. Lee, Y. Krockenberger, K. S. Takahashi, M. Kawasaki, and Y. Tokura, Phys. Rev. B 85, 035101 (2012). 27 G. M. Sheldrick, Acta Crystallogr. Sect. A 64, 112 (2008). 28 Nevill Mott, Metal-Insulator Transition (Taylor & Francis, London, 1990), p. 52.

125105-6